- Nano Express
- Open Access
Enhanced Photoelectrochemical Activity of ZnO-Coated TiO2 Nanotubes and Its Dependence on ZnO Coating Thickness
© Cai et al. 2016
- Received: 23 November 2015
- Accepted: 14 February 2016
- Published: 24 February 2016
One-dimensional heterogeneous nanostructures in the form of ZnO-coated TiO2 nanotubes (ZnO/TiO2 NTs) were fabricated by atomic layer deposition of an ultrathin ZnO coating on electrochemical anodization-formed TiO2 nanotubes (NTs) with the thickness of ZnO coating being precisely controlled at atomic scale, and the photoelectrochemical activity of the fabricated ZnO/TiO2 NTs and the influence of ZnO coating and its thickness were studied. The structures of TiO2 NTs and ZnO coatings were characterized by X-ray diffraction, Raman backscattering spectroscopy, and transmission electron microscopy. The photoelectrochemical activity was studied through the measurements of electrochemical impendence, flat-band potential, and transient photocurrent density. The TiO2 NTs exhibit anatase structure, and the ZnO coatings are structured with hexagonal wurtzite. The photoelectrochemical activity of the ZnO/TiO2 NTs is strongly dependent on the thickness of ZnO coating. ZnO/TiO2 NTs with a thinner rather than a thicker ZnO coating exhibit better photoelectrochemical activity with reduced charge transfer resistance, increased negative flat-band potentials, and enhanced photocurrent densities. Under visible illumination, an increase of about 60 % in the photoelectrochemical activity is obtained for ZnO/TiO2 NTs with an about 2-nm-thick ZnO coating.
- Photoelectrochemical activity
- Heterogeneous nanostructure
- ZnO-coated TiO2 nanotube
Titania (TiO2) and zinc oxide (ZnO) have recently attracted much attention because of their excellent optical, photoelectronic, and photoelectrochemical properties and consequently their potential applications in wide fields including photocatalytic reactions and photovoltaic processes [1–5]. Both metal oxides also have advantages of low cost, physical and chemical stability, nontoxicity, and ease of availability. In addition, TiO2 and ZnO have similar band-gap energies (~3.22 eV for TiO2 and ~3.37 eV for ZnO) and are compatible to each other to compose heterogeneous materials. A variety of heterostructured materials composed of TiO2 and ZnO (TiO2-ZnO) have been reported. Heterogeneous TiO2-ZnO materials exhibit improved individual and combined properties which are very distinct from those of the single constituting materials TiO2 and ZnO and are promising for applications such as photocatalytic reactions and photovoltaic processes. Dye-sensitized solar cells using ZnO-coated nanocrystalline TiO2 films as electrodes, for example, have shown enhanced conversion efficiencies . In particular for heterostructured TiO2-ZnO, nanoscaled TiO2 and ZnO are superior to bulk and film materials in their large surface-to-volume ratio for a large interface between TiO2 and ZnO. Therefore, nanosized heterostructures constructed of nanoscaled TiO2 and ZnO show better photoelectronic, photochemical, and photoelectrochemical properties. When used as a photocatalyst or a photoelectrode, for example, heterogeneous ZnO-TiO2 nanostructures can provide improved performance due to the combination of the high activity of TiO2 with the high electron mobility of ZnO. Furthermore, the alignment of the staggered band gaps of TiO2 and ZnO is favorable for the separation of electrons and holes and consequently the suppression of electron-hole recombination [7, 8]. The staggered band alignment also results in an extension for spectral range of photoresponse, which allows an efficient use of light with a wide spectral band [9, 10]. Therefore, better electrochemical and photoelectrochemical properties and hence enhanced photocatalytic activities and increased photovoltaic efficiencies can be expected for the heterogeneous ZnO-TiO2 nanostructures because of their improved charge conductivity, enhanced charged carrier separation, and extended photoresponse range [11, 12]. Of the diverse ZnO-TiO2 nanoheterostructures, one-dimensional (1D) nanogeometry has received particular attention in the photocatalytic and photovoltaic applications due to its superior charge transport ability and short recombination pathway, which significantly suppresses the recombination of photogenerated electrons and holes [13–16]. The ultraviolet (UV) photoconductivity and photosensitivity of TiO2-coated ZnO nanorods have been reported to be largely enhanced . Using ZnO-sheathed TiO2 as photoanodes, dye-sensitized solar cells have shown enhanced performance . ZnO-coated TiO2 nanotube (ZnO/TiO2 NT) is one of the most studied 1D heterogeneous ZnO-TiO2 nanostructures [16, 19–21]. However, the optimized photocatalytic activity and photovoltaic efficiency of heterogeneous TiO2-ZnO materials including 1D heterogeneous ZnO-TiO2 nanostructures are strongly dependent on the morphology and geometry.
In comparison to bare TiO2 NTs, TiO2 NTs covered by a thin ZnO coating usually present improved electrochemical and photoelectrochemical properties and are expected to have high quantum efficiencies for photocatalytic reactions and photovoltaic processes [16, 19–21]. As a nanoscaled heterostructure, it has been proved that the properties of ZnO/TiO2 NTs are strongly dependent on the geometry and morphology of the heterogeneous nanostructure, the crystal structure of TiO2 and ZnO, and the interfacial quality between TiO2 and ZnO. In the present work, ZnO/TiO2 NTs were fabricated by atomic layer deposition (ALD) of a ZnO coating on the walls of electrochemically anodized TiO2 NTs, and the thickness of ZnO coating was precisely controlled at a sub-nanometer level by varying the growth cycle of ZnO during the ALD process. The properties of the fabricated ZnO/TiO2 NTs and their dependence on the ZnO coating thickness were studied for optimizing the electrochemical and photoelectrochemical activities.
The thickness of the deposited ZnO coating was precisely controlled by ALD growth cycles with 1 cycle of 0.5-s DEZ pulse, 2-s N2 purge, 0.5-s H2O pulse, and 2-s N2 purge. Several sample groups of ZnO/TiO2 NTs were prepared with the same TiO2 NTs but different ZnO coating thickness. Two of them, one with a 10-cycle deposit of ZnO coating (refereed as 10-cycle ZnO/TiO2 NTs) and the other with a 25-cycle deposit of ZnO coating (refereed as 25-cycle ZnO/TiO2 NTs), were compared in this work for a study of the influence of ZnO coating thickness on the properties including photoelectrochemical activity. The obtained heterogeneous nanostructured ZnO-coated TiO2 NTs samples were rinsed with deionized water and annealed at 450 °C for 30 min in air.
The sample morphology was examined by field-emission scanning electron microscopy (FESEM) with a Hitachi S-4800 microscope. The morphology and microstructure of the samples was characterized with a transmission electron microscope (TEM, Tecnai G2 F20 S-Twin). The composition and thickness of the ZnO coatings were evaluated by Rutherford backscattering (RBS) method using a 2.0-MeV He+ beam at 165 ° scattering geometry. The He+ beam generated by a 9SDH-2 tandem accelerator at Fudan University was collimated to a diameter of 1.0 mm for RBS measurements. The structure of the samples was characterized by X-ray diffraction (XRD) with a Rigaku D/max-γ B X-ray diffractometer using a Ni-filtered Cu Kα radiation. The sample structure was also characterized through the analysis of vibrational modes by means of Raman backscattering spectroscopy which was performed with a Jobin-Yvon LabRAM HR 800 UV micro-Raman spectrometer using a 325-nm He–Cd laser light to excite the samples. UV–visible absorption spectra of the samples were recorded with a UV–visible spectrophotometer (Shimadzu UV-350) using a diffuse reflectance integrating sphere.
Photoluminescence (PL) measurements were carried out at room temperature (300 K) and a reduced temperature of 20 K by exciting the samples with a nonpolarized 325-nm He–Cd laser beam, dispersing the emitted luminescence with a 0.5-m spectrometer (Spectra Pro 500i, Acton), and recording the PL spectra with an intensified charge-coupled device (ICCD, iStar DH720, Andor). The spot size of the 325-nm laser beam exciting the samples for PL measurement is about 1 mm in diameter. The electrochemical properties of the samples were studied by electrochemical impedance and flat-band potential measurements using a Potentionstat/Galvanostat (EG & G, 273 A) and a two-phase lock-in amplifier (EG & G, 5210). In a three-electrode cell with a 0.5 M Na2SO4 solution, the impedance measurements were carried out at 0.0 V versus the reference electrode Ag/AgCl with frequencies ranging from 100 kHz to 0.1 Hz, and the flat-band potentials of the samples were determined from the Mott–Schottky plots obtained by measuring at 100 Hz with potentials scanning from 1.0 to 1.5 V at 50 mV/s. Linear-sweep cyclic voltammetry was performed at a potential ranging from +1.5 to −1.5 V versus Ag/AgCl in 0.5 M Na2SO4 at a scan rate of 50 mV/s. With an active area of 1 cm2, the samples were used as photoelectrodes and subjected to intermittent irradiation of visible light (100 mW/cm2) for photocurrent (PC) density measurements in the three-electrode cell in 0.5 M Na2SO4 using a CHI electrochemical analyzer (CHI 660A). A 500-W xenon lamp was used as the light source to provide visible light by removing infrared light with a quartz wafer filter and cutting ultraviolet (UV) light using a high-pass filter with a cutoff of 380 or 420 nm.
Raman backscattering measurements confirm the anatase structure of the TiO2 NTs and the wurtzite structure of the ZnO coatings, as shown in Fig. 3b. The Raman spectrum taken from the bare TiO2 NTs exhibits three distinct peaks located at 392, 514, and 633 cm−1, respectively. They are attributed to the characteristic Raman reactive B1g mode, doublet A1g/B1g mode, and Eg mode of anatase TiO2 [27, 28]. In addition, a broad band centered near 820 cm−1 is resolved, which is attributed to the B2g mode of rutile TiO2. In the Raman spectrum taken from the bare TiO2 NTs, A and R in parentheses denote the anatase and the rutile phase of TiO2, respectively. After being covered by a 10- or 25-cycle deposit of ZnO coating, the above TiO2 modes are greatly suppressed and the Raman spectra are predominated by three strong backscattering peaks at 574, 1147, and 1720 cm−1. The strongest peak at 574 cm−1 is attributed to the polar optical mode associated with longitudinal optical (LO) phonons of ZnO [A1(LO)], while the other two peaks at 1147 and 1720 cm−1 are the overtones of A1(LO) and result from 2- and 3-phonon scattering processes [A1(2LO) and A1(3LO)], respectively [29, 30]. The reduction in the measured Raman signals scattered from TiO2 for the ZnO-coated TiO2 nanotubes is mainly attributed to the absorption of the photons in the exciting 325-nm light by the ZnO coating.
Generally, the PL from the sample becomes stronger at low temperatures. The inset in Fig. 6a compares the PL spectra of the 25-cycle ZnO/TiO2 NTs measured at 300 and 20 K, respectively. At 20 K, the intensity of the UV ZnO NBE luminescence is increased about one order of magnitude for the 25-cycle ZnO/TiO2 NTs as a result of the freezing of phonons and the quenching of nonradiative recombination processes at low temperatures [30, 35, 39]. The UV ZnO NBE luminescence at low temperature is still without the company of defect-related visible emission, but with a narrowed width as compared to that recorded at room temperature, as shown in Fig. 6b which illustrates the PL spectra recorded at 20 K. For the bare TiO2 NTs, only the defect-related visible emission is observed. In addition to the defect-related visible emission, the PL of the 10-cycle ZnO/TiO2 NTs includes a weak UV NBE luminescence from the ZnO coating with its intensity less than 2 % of that of the 25-cycle ZnO/TiO2 NTs. The comparison of the PL spectra of the ZnO-coated TiO2 NTs with that of the bare TiO2 NTs, measured at room temperature and low temperature, suggests that the visible emission is most probable associated with the defects in TiO2 NTs. Moreover, the much weak PL from the 10-cycle ZnO/TiO2 NTs as compared to that from the 25-cycle ZnO/TiO2 NTs reveals a lower rate of radiative recombination of photogenerated electrons and holes in the 10-cycle deposit of ZnO than in 25-cycle deposit of ZnO, implying that ZnO/TiO2 NTs with a thinner rather than a thicker ZnO coating have more efficient spatial separation of photogenerated electrons and holes and hence exhibit better photoelectrochemical activity as will be described below.
The flat-band potentials of the TiO2 NTs and ZnO/TiO2 NTs electrodes were determined by the Mott–Schottky analysis method [41, 42]. Figure 7b displays the Mott–Schottky plots of the bare TiO2 NTs and the ZnO-coated TiO2 NTs. The reversed sigmoidal plots with an overall shape are consistent with that typical for n-type semiconductors . In addition, the reproducible flat-band potentials, i.e., the potentials corresponding to the situation in which there is no charge accumulation in the semiconductor so that the energy bands experience no bending can be obtained by intersecting the tangent of Mott–Schottky curves with the potential axis. The flat-band potential (V fb) for the 10-cycle ZnO-coated TiO2 NTs shifts negatively to −0.53 V from −0.42 V for the bare TiO2 NTs, revealing a smaller barrier for charge transfer in the 10-cycle ZnO/TiO2 NTs. The thin ZnO coating on the TiO2 surface forms an inherent barrier layer to block electron transfer from the conduction band or trap sites of TiO2 to electrolyte, retarding charge recombination in the TiO2/electrolyte interface . The V fb plays an important role in photoelectrochemical performance. A more negative V fb suggests a higher photoelectrochemical activity. When used as the photoelectrode in a photovoltaic device, for example, a higher open-circuit voltage can be expected, since the open-circuit voltage (V oc) of a photovoltaic device is generally determined by the offset between the quasi Fermi level of electrodes and the redox level of electrolyte . However, the 25-cycle ZnO-coated TiO2 NTs present a smaller negative value of V fb, even smaller than that of the bare TiO2 NTs. This can also be attributed to the higher recombination rate in thicker ZnO coating.
The increased PC density and the enhanced photoelectrochemical activity can also be ascribed to a large number of electron-hole pairs formed under the illumination of the light around 380 nm the energy of whose photons is nearly resonant with the band gap of ZnO. As described above, however, the presence of the ZnO coatings on the TiO2 NTs results in a red shift of absorption edge and allows the ZnO-coated TiO2 NTs to absorb visible light. In order to investigate the influence of the ZnO coverage on the photoelectrochemical activity under visible illumination, PC measurements were also performed under intermittent visible illumination with a wavelength cutoff of 420 nm. Although the corresponding PC densities are generally lower than those obtained under the illumination with the wavelength cutoff of 380 nm, the ZnO-covered TiO2 NTs present enhanced photoelectrochemical activities compared with the bare TiO2 NTs. For the 10-cycle ZnO-covered TiO2 NTs, in particular, a significant enhancement of photoelectrochemical activity is observed. The PC density increases from ~1.4 μA/cm2 for the bare TiO2 NTs to ~2.2 μA/cm2 for the 10-cycle ZnO/TiO2 NTs, as shown in Fig. 9b. An increase of nearly 60 % in photoelectrochemical activity is therefore obtained for the TiO2 NTs covered by a 10-cycle deposit of ZnO, or by a 2.1-nm ZnO coating, compared with the bare TiO2 NTs. In contrast, the 25-cycle ZnO/TiO2 NTs just show a slight increase of PC density compared with the bare TiO2 NTs. One of the factors unfavorable for the enhancement in the photoelectrochemical activity of the 25-cycle ZnO/TiO2 NTs should be the thicker ZnO coating, which presents a longer pathway for the generated electrons to migrate to the TiO2 surface and the generated holes to the ZnO surface, and hence increases the recombination of electrons and holes, not conducive to the separation of electrons and holes. Apparently, the higher photoelectrochemical activity of the 10-cycle ZnO/TiO2 NTs is consistent with the suppressed recombination of electrons and holes in the heterogeneous nanostructures composed of TiO2 NTs and ultrathin ZnO coating. The above results suggest that from the view of enhancing photoelectrochemical activity, ZnO coatings of about 2 nm in thickness are optimal for heterostructured ZnO/TiO2 NTs [19, 40, 48, 49].
Vertically aligned ZnO-coated TiO2 NTs were fabricated by ALD deposition of ultrathin ZnO coatings on the walls of the TiO2 NTs formed by electrochemical anodization of Ti foils. The TiO2 NTs exhibit anatase structure while the ZnO coatings are structured with hexagonal wurtzite with precise thickness control at atomic scale for an investigation on the influence of ZnO coating and its thickness on the optical, electrochemical, and photoelectrochemical properties of the heterogeneous nanostructured ZnO/TiO2 NTs. The fabricated bare TiO2 NTs and the ZnO-coated TiO2 NTs present fast photoresponse and good photostability. Compared with bare TiO2 NTs, the presence of ZnO coatings significantly improves the electrochemical and photoelectrochemical activities due to the enhanced charge separation in the heterostructure composed of TiO2 NTs and ZnO coatings, especially the TiO2 NTs covered by a thinner ZnO coating of about 2 nm in thickness rather than a thicker ZnO coating. In comparison to the bare TiO2 NTs, an increase of nearly 60 % in photoelectrochemical activity is obtained for the TiO2 NTs covered by an about 2-nm-thick ZnO coating under visible illumination with a wavelength cutoff of 420 nm.
This work is supported by the National Natural Science Foundation of China (11275051). Acknowledgment is also made to the Municipal Natural Science Foundation of Shanghai (15ZR1403300).
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Khan SUM, Al-Shahry M, Ingler WB (2002) Efficient photochemical water splitting by a chemically modified n-TiO2. Science 297:2243–5View ArticleGoogle Scholar
- Mor GK, Shankar K, Paulose M, Varghese OK, Grimes CA (2006) Use of highly-ordered TiO2 nanotube arrays in dye-sensitized solar cells. Nano Lett 6:215–8View ArticleGoogle Scholar
- Rensmo H, Keis K, Lindstroem H, Sodergren S, Solbrand A, Hagfeldt A, Lindquist SE, Wang LN, Muhammed M (1997) High light-to-energy conversion efficiencies for solar cells based on nanostructured ZnO electrodes. J Phys Chem B 101:2598–601View ArticleGoogle Scholar
- Zhang QF, Dandeneau CS, Zhou XY, Cao GZ (2009) ZnO nanostructures for dye-sensitized solar cells. Adv Mater 1:4087–108View ArticleGoogle Scholar
- Law M, Greene LE, Johnson JC, Saykally R, Yang PD (2005) Nanowire dye-sensitized solar cells. Nat Mater 4:455–9View ArticleGoogle Scholar
- Susmitha K, Kumar MN, Rajkumar G, Giribabu L, Raghavender M (2015) Enhanced dye sensitized solar cell performance with high surface area thin ZnO film and PEDOT:PSS. Sol Energy 118:126–33View ArticleGoogle Scholar
- van Embden J, Jasieniak J, Gomez DE, Mulvaney P, Giersig M (2007) Review of the synthetic chemistry involved in the production of core/shell semiconductor nanocrystals. J Chem 60:457–71Google Scholar
- Roh SJ, Mane RS, Min SK, Lee WJ, Lokhande CD, Han SH (2006) Achievement of 4.51 % conversion efficiency using ZnO recombination barrier layer in TiO2 based dye-sensitized solar cells. Appl Phys Lett 89:253512, 1−3View ArticleGoogle Scholar
- Reiss P, Protiere M, Li L (2009) Core/shell semiconductor nanocrystals. Small 5:154–68View ArticleGoogle Scholar
- Wu ZM, Zhang Y, Zheng JJ, Lin XG, Chen XH, Huang BW, Wang HQ, Huang K, Li SP, Kang JY (2011) An all-inorganic type-II heterojunction array with nearly full solar spectral response based on ZnO/ZnSe core/shell nanowires. J Mater Chem 21:6020–6View ArticleGoogle Scholar
- Pan L, Shen GQ, Zhang JW, Wei XC, Wang L, Zou JJ, Zhang XW (2015) TiO2-ZnO composite sphere decorated with ZnO clusters for effective charge isolation in photocatalysis. Ind Eng Chem Res 54:7226–32View ArticleGoogle Scholar
- Kayaci F, Vempati S, Ozgit-Akgun C, Donmez I, Biyikli N, Uyar T (2014) Selective isolation of the electron or hole in photocatalysis: selective isolation of the electron or hole in photocatalysis: ZnO–TiO2 and TiO2–ZnO core–shell structured heterojunction nanofibers via electrospinning and atomic layer deposition. Nanoscale 6:5735–45View ArticleGoogle Scholar
- Ji IA, Park MJ, Jung JY, Choi MJ, Lee YW, Lee JH, Bang JH (2012) One-dimensional core/shell structured TiO2/ZnO heterojunction for improved photoelectrochemical performance. Bull Korean Chem Soc 33:2200–6View ArticleGoogle Scholar
- Momeni MM, Ghayeb Y (2015) Visible light-driven photoelectrochemical water splitting on ZnO-TiO heterogeneous nanotube photoanodes. J Appl Electrochem 45: 557–566.View ArticleGoogle Scholar
- Amna T, Hassan MS, Khil MS, Lee HK, Hwang IH (2014) Electrospun nanofibers of ZnO-TiO2 hybrid: characterization and potential as an extracellular scaffold for supporting myoblasts. Surf Interface Anal 46:72–6View ArticleGoogle Scholar
- Liu R, Yang WD, Qiang LS, Liu HY (2012) Conveniently fabricated heterojunction ZnO/TiO2 electrodes using TiO2 nanotube arrays for dye-sensitized solar cells. J Power Sources 22:153–9View ArticleGoogle Scholar
- Panigrahi S, Basak D (2011) Core-shell TiO2@ZnO nanorods for efficient ultraviolet photodetection. Nanoscale 3:2336–41View ArticleGoogle Scholar
- Ulusoy TG, Ghobadiac A, Okyay AK (2014) Surface engineered angstrom thick ZnO-sheathed TiO2 nanowires as photoanodes for performance enhanced dye-sensitized solar cells. J Mater Chem A 2:16867–76View ArticleGoogle Scholar
- Shaheen BS, Salem HG, El-Sayed MA, Allam NK (2013) Thermal/electrochemical growth and characterization of one-dimensional ZnO/TiO2 hybrid nanoelectrodes for solar fuel production. J Phys Chem C 117:18502–9View ArticleGoogle Scholar
- Jeong JS, Choe BH, Lee JH, Lee JJ, Choi WY (2014) ZnO-coated TiO2 nanotube arrays for a photoelectrode in dye-sensitized solar cells. J Electron Mater 43:375–80View ArticleGoogle Scholar
- Cai H, Yang Q, Hu ZG, Duan ZH, You QH, Sun J, Xu N, Wu JD (2014) Enhanced photoelectrochemical activity of vertically aligned ZnO-coated TiO2 nanotubes. Appl Phys Lett 104:053114, 104View ArticleGoogle Scholar
- Cai H, You QH, Hu ZG, Duan ZH, Cui Y, Sun J, Xu N, Wu JD (2014) Fabrication and correlation between photoluminescence and photoelectrochemical properties of vertically aligned ZnO coated TiO2 nanotube array. Sol Energy Mater Sol Cells 123:233–8View ArticleGoogle Scholar
- Ott AW, Chang RPH (1999) Atomic layer-controlled growth of transparent conducting ZnO on plastic substrates. Mater Chem Phys 58:132–8View ArticleGoogle Scholar
- Zhao JQ, Wang Y (2012) Ultrathin surface coatings for improved electrochemical performance of lithium ion battery electrodes at elevated temperature. J Phys Chem C 116:11867–76View ArticleGoogle Scholar
- Mayer M (1997) SIMNRA user’s guide. Max-Planck-Institut für Plasmaphysik, Garching, Tech. Rep. IPP 9/113Google Scholar
- Geng Y, Guo L, Xu SS, Sun QQ, Ding SJ, Lu HL, Zhang DW (2011) Influence of Al doping on the properties of ZnO thin films grown by atomic layer deposition. J Phys Chem C 115:12317–21View ArticleGoogle Scholar
- Porto SPS, Fleury PA, Damen TC (1967) Raman spectra of TiO2, MgF2, ZnF2, FeF2, and MnF2. Phys Rev 154:522–4View ArticleGoogle Scholar
- Ohsaka T, Izumi F, Fujiki Y (1978) Raman spectrum of anatase TiO2. J Raman Spectrosc 7:321–4View ArticleGoogle Scholar
- Scott JF (1970) UV resonant Raman scattering in ZnO. Phys Rev B 2:1209–11View ArticleGoogle Scholar
- Li Q, Gao K, Hu ZG, Yu WL, Xu N, Sun J, Wu JD (2012) Photoluminescence and lasing properties of catalyst-free ZnO nanorod arrays fabricated by pulsed laser deposition. J Phys Chem C 116:2330–5View ArticleGoogle Scholar
- Hernandez S, Cauda V, Chiodoni A, Dallorto S, Sacco A, Hidalgo D, Celasco E, Pirri CF (2014) Optimization of 1D ZnO@TiO2 core-shell nanostructures for enhanced photoelectrochemical water splitting under solar light illumination. ACS Appl Mater Interfaces 6:12153–67View ArticleGoogle Scholar
- Yan XD, Zou CW, Gao XD, Gao W (2012) ZnO/TiO2 core–brush nanostructure: processing, microstructure and enhanced photocatalytic activity. J Mater Chem 22:5629–40View ArticleGoogle Scholar
- Vanheusden K, Warren WL, Seager CH, Tallant DK, Voigt JA, Gnade BE (1996) Mechanisms behind green photoluminescence in ZnO phosphor powders. J Appl Phys 79:7983–9View ArticleGoogle Scholar
- Li D, Leung YH, Djurisic AB, Liu ZT, Xie MH, Shi SL, Xu SJ, Chan WK (2004) Different origins of visible luminescence in ZnO nanostructures fabricated by the chemical and evaporation methods. Appl Phys Lett 85:1601–3View ArticleGoogle Scholar
- Shan W, Walukiewicz W, Ager JW III, Yu KM, Yuan HB, Xin HP, Cantwell G, Song JJ (2005) Nature of room-temperature photoluminescence in ZnO. Appl Phys Lett 86:191911, 1−3View ArticleGoogle Scholar
- Zhang BP, Binh NT, Segawa Y, Wakatsuki K, Usami N (2003) Optical properties of ZnO rods formed by metalorganic chemical vapor deposition. Appl Phys Lett 83:1635–7View ArticleGoogle Scholar
- Chang YH, Liu CM, Chen C, Cheng HE (2012) The effect of geometric structure on photoluminescence characteristics of 1-D TiO2 nanotubes and 2-D TiO2 films fabricated by atomic layer deposition. J Electrochem Soc 159:D401–5View ArticleGoogle Scholar
- Zhang JF, Zhou P, Liu JJ, Yu JG (2014) New understanding of the difference of photocatalytic activity among anatase, rutile and brookite TiO2. Phys Chem Chem Phys 16:20382–6View ArticleGoogle Scholar
- Ko HJ, Chen YF, Zhu Z, Yao T, Kobayashi I, Uchiki H (2000) Photoluminescence properties of ZnO epilayers grown on CaF2(111) by plasma assisted molecular beam epitaxy. Appl Phys Lett 76:1905–7View ArticleGoogle Scholar
- Chandiran AK, Abdi-Jalebi M, Nazeeruddin MK, Grätze M (2014) Analysis of electron transfer properties of ZnO and TiO2 photoanodes for dye-sensitized solar cells. ACS Nano 8:2261–8View ArticleGoogle Scholar
- Cardon F, Gomes WP (1978) On the determination of the flat-band potential of a semiconductor in contact with a metal or an electrolyte from the Mott-Schottky plot. J Phys D Appl Phys 11:L63–7View ArticleGoogle Scholar
- Seungho S, Jang JW, Park YB, Kim JY, Magesh G, Kim JH, Seol M, Yong K, Lee KH, Lee JS (2014) An exceptionally facile method to produce layered double hydroxides on a conducting substrate and their application for solar water splitting without an external bias. Energy Environ Sci 7:2301–7View ArticleGoogle Scholar
- Kang SH, Kim JY, Kim Y, Kim HS, Sung YE (2007) Surface modification of stretched TiO2 nanotubes for solid-state dye-sensitized solar cells. J Phys Chem C 111:9614–23View ArticleGoogle Scholar
- Wu DP, Gao ZY, Xu F, Shi ZP, Tao WG, Jiang K (2012) Nanosheet-based hierarchical ZnO structure decorated with TiO2 particles for enhanced performance in dye-sensitized solar cell. Cryst Eng Comm 14:7934–41View ArticleGoogle Scholar
- Xiao FX (2012) Construction of highly ordered ZnO–TiO2 nanotube arrays (ZnO/TNTs) heterostructure for photocatalytic application. ACS Appl Mater Interfaces 4:7055–63View ArticleGoogle Scholar
- Bai XD, Wang EG, Gao PX, Wang ZL (2003) Measuring the work function at a nanobelt tip and at a nanoparticle surface. Nano Lett 3:1147–50View ArticleGoogle Scholar
- Xiong G, Shao R, Droubay TC, Joly AG, Beck KM, Chambers SA, Hess WP (2007) Photoemission electron microscopy of TiO2 anatase films embedded with rutile nanocrystals. Adv Funct Mater 17:2133–8View ArticleGoogle Scholar
- Cheun H, Fuentes-Hernandez C, Zhou YH, Potscavage WJ, Kim SJ, Shim J, Dindar A, Kippelen B (2010) Electrical and optical properties of ZnO processed by atomic layer deposition in inverted polymer solar cells. J Phys Chem C 114:20713–8View ArticleGoogle Scholar
- Greene LE, Law M, Yuhas BD, Yang PD (2007) ZnO-TiO2 core-shell nanorod/P3HT solar cells. J Phys Chem C 111:18451–6View ArticleGoogle Scholar